ANALYSIS OF FRICTION STIR WELDING PROCESS FOR 304L STAINLESS STEEL
Swapnil J. More and2*
VIVA institute of Technology Shirgaon, Veer Sawarkar road, Virar (East), Tal- Vasai,
Dist-Thane, Maharashtra, India
Faculty of Engineering, University of Mumbai, India
This paper focusses on Friction stir welding (FSW) invented by Wayne Thomas in The Welding Institute (TWI) at London in 1991. Friction stir welding (FSW) is a solid state joining process which means joining of metal plates without reaching the melting point of the material to be welded. FSW uses a non-consumable rotating tool which is plunged into workpiece material due to which heat is generated between tool shoulder and workpiece surface which results in plastic deformation of material to be welded. This technique of joining metal is energy efficient, environmental friendly and can be used to join high strength aluminium alloys and other alloys that are hard to weld by conventional fusion welding. The paper focuses on performing simulation using Ansys for joining 304L stainless steel plates, to obtain better quality of welds by varying the input process variables.
Copyright © 2016Swapnil J. More and Niyati Raut.This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
The heat transfer process is one of the most important aspects in the FSW study. A good understanding of the heat transfer process in the work piece can be helpful in predicting the thermal cycles in the welding work piece, and the hardness in the weld zone, subsequently, can be helpful in evaluating the weld quality. In this process, the heat is originally derived from the friction between the welding tool (including the shoulder and the probe) and the welded material, which causes the welded material to soften at a temperature less than its melting point. The softened material underneath the shoulder is further subjected to extrusion by the tool rotational and transverse movements. It is expected that this process will inherently produce a weld with less residual stress and distortion as compared to the fusion welding methods, since no melting of the material occurs during the welding. Despite significant advances in the application of FSW as a relatively new welding technique for welding, the fundamental knowledge of thermal impact and thermo mechanical processes are still not completely understood. To study the variations of transient temperature and frictional heat developed in friction stir welding of 304L stainless steel plates, detailed three-dimensional nonlinear thermal and thermo-mechanical simulations are performed for the FSW process using Ansys
*Corresponding author: Niyati Raut,
VIVA institute of Technology Shirgaon, Veer Sawarkar road, Virar (East), Tal- Vasai, Dist-Thane, Maharashtra, India.
APDL by varying input process variables tool rotational speed and tool linear velocity. Simulation of FSW process is carried out using Ansys APDL. A nonlinear direct coupled-field analysis is performed, as thermal and mechanical behaviours are mutually dependent and coupled together during the FSW process. Because the temperature field affects stress distribution a fully thermo-mechanically coupled model is created. The model consists of a coupled-field solid element with structural and thermal degrees of freedom. The model has two rectangular steel plates and a cylindrical tool. All necessary mechanical and thermal boundary conditions are applied on the model. The simulation occurs over three load steps, representing the plunge, dwell, and traverse phases of the process. The temperature rises at the contact interface due to frictional contact between the tool and workpiece. FSW generally occurs when the temperature at the weld line region reaches 70 to 90 percent of the melting temperature of the work piece material. The temperature obtained around the weld line region in this analysis falls within the range reported by Zhu and Chao, while the maximum resulting temperature is well below the melting temperature of the workpiece. A bonding temperature is specified at the contact interface of the plates to model the welding behind the tool. When the temperature at the contact surface exceeds this bonding temperature, the contact is changed to bonded. The tool pin is ignored. The heat generated at the pin represents approximately two percent of the total heat and is therefore negligible. The FSW process generally requires a tool made of
ISSN: 0976-3376Asian Journal of Science and Technology Vol.07, Issue, 04, pp.2769-2773, April, 2016
ASIAN JOURNAL OF
SCIENCE AND TECHNOLOGY
Article History: Received 26th January, 2015 Received in revised form 14th February, 2016 Accepted 08th March, 2016 Published online 27th April, 2016
Friction stir welding (FSW), 304L stainless steel, Nonlinear analysis,
a harder material than the workpiece material being welded. In the past, FSW was used for soft workpiece materials such as aluminium, with the development of tools made from super-abrasive materials such as polycrystalline cubic boron nitride (PCBN), FSW has become possible with high-temperature materials such as stainless steel. A cylindrical PCBN tool is modeled in this case. The workpiece sides parallel to the weld line are constrained in all the directions to simulate the clamping ends. The bottom side of the workpiece is constrained in the perpendicular (z) direction to simulate support at the bottom. Heat losses are considered on all the surfaces of the model. All boundary conditions are symmetric across the weld centerline. The simulation is performed in three load steps, each representing a respective phase (plunge, dwell, and traverse) of the FSW process.
Friction stir welding is latest technology in industry and it has many advantages on traditional welding technologies. Normally metals and alloys are joined by fusion welding process. All fusion welding processes (particularly for materials having low weldability such as copper) are characterized by welding defects and Some metals like Al, Cu and Mg alloy series are not at all fusion weldable. Also Welding of different materials and much different in thickness are impossible/very difficult with fusion welding process. Main drawback of FSW process is that selection of correct input parameters to insure good weld quality. Generally this selection is based on trial and error method. Now the rotational speed, linear travel speed and downward force of the tool are the process parameters which need to be controlled to get good quality of weld. The downward force of the tool is kept constant while the rotational and linear speed is varied for heat generation beneath the tool shoulder. Downward force of the tools helps to achieve proper frictional contact. The selection of other two process parameters are generally selected on trial and error method so the need is to perform simulation to predict the process parameters that are rotational speed and linear speed to achieve good quality of weld and to find out frictional heat developed during welding. Thermomechanical model developed by Zhu and Chao for friction stir welding of 304L stainless steel is replicated using ANSYS. The developed model is then used to conduct parametric studies to understand the effect of various input parameters like rate of tool velocity and tool rotational speed on temperature distribution developed in the work piece.
The objective is to study the effect of tool rotation speed and tool linear velocity on the maximum temperature and frictional heat developed during the welding process. The heat developed during the welding process depends on the friction between tool and the workpiece. In order to achieve good quality welds, weld input parameters such as tool rotational speed, translation velocity, heat input and tool dimensions have to be properly controlled. As the quality of a weld joint is directly influenced by the input parameters, the welding process can be considered as a input, multi-output process. Thus appropriate combinations of weld parameters have to be chosen to produce high quality welds with minimum detrimental residual stresses and distortions. This project focuses on investigation of input parameters that control the welding temperature in 304L stainless steel friction
stir welds and on model-based optimization of the process.
Fig. 1. Layout for model creation and performing analysis using Ansys
Thermo mechanical model of FSW
The Finite Element Method (FEM) offers a way to solve complex continuum problems by subdividing it into a series of simple interrelated problems. FEM is most commonly used in numerical analysis for obtaining approximate solutions to wide variety of engineering problems. In the present study, a
commercial general purpose finite element program ANSYS®
14.5 was used for numerical simulation of friction stir welding process.
The purpose of the thermal model is to calculate the transient temperature fields developed in the workpiece during friction stir welding. In the thermal analysis, the transient temperature field which is a function of time and the spatial coordinates ( ,y,z), is estimated by the three dimensional nonlinear heat transfer equation 1,
t T c Q z
int 2 2 2 2 2 2
Where k is the coefficient of thermal conductivity, Qint is the internal heat source rate, c is the mass-specific heat capacity, ρ
is the density of materials.
A number of assumptions have been made in developing the
finite element thermal model, which include:
Workpiece material is isotropic and homogen
No melting occurs during the welding
Thermal boundary conditions are sy
the weld centerline.
Heat transfer from the workpiece
In the numerical model, only half of the modeled as the weld line is the symmetric condition is used to reduce the simulation tim has dimensions of 0.0762 m x 0.03175 m x shown in Fig 2.
Fig. 2. Geometry of workpiece
In the present thermal analysis, the workpiec a brick element called SOLID 226. This elem dimension thermal conduction capability and
three- dimensional, steady-state or tr
analysis. The element is defined by e temperature as single degree of freedom at the orthotropic material properties. Heat flux (but not both) can be input as surface loads a
Three dimensional SOLID226 elements were used sheets. The workpiece was divided into 22 p length with spacing ratio 5, 44 parts along parts along the thickness direction. The mesh is total number of 5214 elements and 7879 nodes
Boundary condition for FSW thermal model
surface loads through ANSYScodes. Assump
for various boundary conditions based on da various published research papers (Zhu and Convective and radiative heat losses to the across all free surfaces of the workpiece and occur from the workpiece bottom surface to To consider convection and radiation on surfaces except for the bottom, the heat loss q by following equation 2,
nd homogeneous. ng process.
to the clamp is
the welded plate is tric line. Symmetric
me. The workpiece 0.03175 m x 0.00318 m as
Fig. 2. Geometry of workpiece
ce is meshed using lement has a three-nd can be used for a
eight nodes with each node and by xes or convections at the element.
e used to mesh the o 22 parts along the long the width and 2 mesh is comprised of a s and 7879 nodes.
model were specified as Assumptions were made ata collected from and Chao, 2004). the ambient occurs conduction losses the backing plate. on all workpiece t loss qs is calculated
Where, is absolute temperature of the workpiece, ambient temperature, is the convection coefficient, emissivity of the plate surfaces, and
is the Stefan-Boltzmann constant. In the current model, a typical value of was taken to be 10
temperature of 300 K and was taken to be 0.17 for 304L steel. In order to account for the conductive heat loss through the bottom surface of weld plates, a high overall heat transfer coefficient has been assumed. This assumption is based on the
previous studies (Zhu and Chao
heat loss was modeled approximately by using heat flux loss by convection given by following equation 3,
Where is a fictitious convec
Due to the complexity involved in estimating the contact condition between the sheet and the backing plate, the value of had to be estimated by assuming different values through reverse analysis approach. In this study, the optimized value of
was found to be 100 representation of boundary condi
Fig. 3. Schematic representation of boundary thermal analysis
Heat is produced in the friction stir welding process due to the friction between the tool shoulder and workpiece interface and due to the plastic deformation of the model weld metal near the pin. The heat generated by the plastic deformation of weld metal near the pin is of negligible magnitude and is difficult to quantify (Yuh et al., 2003). Hence, it was neglected in this study. Therefore in this, the heat generated by friction between the workpiece and tool shoulder is the only source of heat generation. The total heat input
calculated through (Yuh et al.,
as a moving heat flux. The total heat input following equation 4,
i o i i o o
Where, is the tool rotational speed, coefficient, is the downward force, the shoulder and the nib of the pin tool. to the workpiece q(r) is assumed to be axis linearly distributed in the radial direction and is calculated by equation 5,
is absolute temperature of the workpiece, 0 is the
is the convection coefficient, is the
emissivity of the plate surfaces, and = 5.67 x 10-12 2℃
Boltzmann constant. In the current model, a
was taken to be 10 2℃ using an ambient
was taken to be 0.17 for 304L In order to account for the conductive heat loss through the bottom surface of weld plates, a high overall heat transfer assumed. This assumption is based on the
Chao, 2004; Yuh et al., 2003). The
heat loss was modeled approximately by using heat flux loss given by following equation 3,
is a fictitious convection coefficient
Due to the complexity involved in estimating the contact condition between the sheet and the backing plate, the value of had to be estimated by assuming different values through ach. In this study, the optimized value of
was found to be 100 / 2℃. Fig. 3 Schematic
ondition for thermal analysis.
Schematic representation of boundary condition for thermal analysis
Heat is produced in the friction stir welding process due to the friction between the tool shoulder and workpiece interface and due to the plastic deformation of the model weld metal near the pin. The heat generated by the plastic deformation of weld near the pin is of negligible magnitude and is difficult to Hence, it was neglected in this study. Therefore in this, the heat generated by friction between the workpiece and tool shoulder is the only source of heat The total heat input in watts for this model is
et al., 2003) equation and is applied
as a moving heat flux. The total heat input is given by
is the tool rotational speed, is the frictional is the downward force, o and i are the radii of
the shoulder and the nib of the pin tool. The rate of heat input to the workpiece q(r) is assumed to be axis-symmetric and ributed in the radial direction (Yuh et al., 2003)
In the present simulation, the heat flux q(r) obtained from the above equation is applied as surface load using tabular boundary condition. The movement of FSW tool is implemented by creating a local cylindrical coordinate system and calculating heat load at each node at each instantaneous time step. The dimensions for tool and values for other parameters used in this study were obtained from (Zhu and Chao, 2004) for correlation to the published research data. The tool shoulder diameter used in this study was 19.05 mm, while the pin diameter was assumed as zero. The assumption was made based on findings from Russell and Sheercliff that the heat generated at the pin of the tool is in the order of 2% of
total heat and hence negligible. Fitted values of and were
used in this study.
The following assumptions have been made in developing the structural model:
Deformation occurs symmetrically along the weld
line, so only half of the workpiece is modeled.
The plate material is homogeneous.
The effect of creep is neglected because there is no
cyclic thermal load involved.
RESULTS AND DISCUSSION
The values of input parameters are increased by 10% and the results were plotted.
First analysis with 60 rpm and 2.71 mm/s tool velocity
Graph 4.1 Temperatures vs. Time (60 rpm)
It is observed that temperature slowly increases with time. It reaches maximum temperature at 18 sec after the process started and corresponding temperature is 1300oc.
Graph 4.2 Frictional heat vs. Time (60 rpm)
Friction between tool and the workpiece generate heat. The maximum temperature generated due to friction is about 820oJ. (Graph 4.2)
Analysis with 66 rpm and 2.71 mm/s tool velocity
Graph 4.3 Temperatures vs. Time (66 rpm)
The Temperature variations are shown in the graph. For first few seconds the temperature increases linearly, after 4 sec there is sudden decrement in the welding temperature. After 7 seconds temperature rises.
Graph 4.4 Frictional heat vs. Time (66 rpm)
Fiction heat is increases with time but is will slightly decreases at the end of the process.
Analysis with 78 rpm and 2.71 mm/s tool velocity
Graph 4.5 Temperatures vs. Time (78 rpm)
For first few seconds temperature increases linearly then there is sudden drop in the temperature. The temperature achieve during initial stage is the maximum temperature.
Graph 4.6 Frictional heat vs. Time (78 rpm) Maximum friction heat is between 900 to 1000J.
Non-linear Thermo-coupled analysis was use to find temperature and friction heat in welding process. It is observed that tool rotation speed and tool velocity plays an important role in friction stir welding process.
As the rotation speed of the tool increases, maximum temperature decrease because of increase in convection due to tool rotation.
Increased rotation speed also increases the friction heat
developed between tool and the workpiece.
For better weld we suggest higher tool rotation speed and lower tool velocity.
This work supported by VIVA Institute of Technology, Virar, Maharashtra, India by the Department of Mechanical engineering & Technology.
Bastier, A., Maitournam, M.H., Roger, F., and Van, K.D. 2008. Modelling of the residual state of friction stir welded
plates. Journal of Materials Processing Technology,
200(1-3): p. 25-37.
Cartigueyen, S., O.P. Sukesh, K. Mahadevan, 2014. Numerical and Experimental Investigations of Heat Generation during Friction Stir Processing of Copper. Procedia Engineering
97, 1069 – 1078
Chen, C.M., R. Kovacevic, 2003. Finite element modeling of friction stir welding—thermal and thermomechanical
analysis. International Journal of Machine Tools &
Manufacture 43, 1319–1326
Leonard, A. J. and S. A. Lockyer, 2003. Flaws in Friction stir welding. 4th International Symposium on friction stir welding, Park city, Utah, USA, 14-16 May.
Li, T., Shi, Q.Y., and Li, H.K. 2007. Residual stresses simulation for friction stir welded joint. Science and
Technology of Welding and Joining, 12(8): p. 664-670.
Madhavi, B., J. Jeevan and M. Karthik Teja, 2014. Heat and Material Flow Effects on Microstructures and Hardness in
Friction-Stir Welded Joints. Procedia Engineering 86, 209
Mir Zahedul, H., Khandkar, Jamil A. Khan, Anthony, P. Reynolds, Michael A. Sutton, 2006. Predicting residual thermal stresses in friction stir welded metals. Journal of
Materials Processing Technology, 174, 195–203
Muhsin, J. J., Moneer, H. 2012. Tolephih and Muhammed A. M. Effect of friction stir welding parameters(rotation and transverse) speed on the transient temperature distribution
in friction stir welding of AA 7020-T53. ARPN Journal of
Engineering and Applied Sciences, Vol. 7, No. 4, April.
Padmanaban, R., V. Ratna Kishore and V. Balusamy, 2014. Numerical Simulation of Temperature Distribution and Material Flow During Friction Stir Welding of Dissimilar
Aluminum Alloys. Procedia Engineering 97, 854 – 863
Rajakumar, S., C. Muralidharan, V. Balasubramanian, 2010. Influence of friction stir welding process and tool parameters on strength properties of AA7075-T6 aluminium alloy joints, Elsevier.
Selvaraj, M. 2013. A temperature dependent slip factor based thermal model for friction stir welding of stainless steel, Sadhana Vol. 38, Part 6, December, pp.
1393–1405. Indian Academy of Sciences.
Sergio Neves Monteiro, Ana Lucia Diegues Skury, Marcia
Giardinieri de Azevedo, Guerold Sergueevitch
Bobrovnitchii, 2013. Cubic boron nitride competing with diamond as a superhard engineering material – an overview, Journal of material research and technology, 2(1): 68-74
Song, M. and R. Kovacevic, 2003. Thermal modelling of friction stir welding in a moving coordinate system and its validation. International Journal of Machine Tools and
Manufacture 43, 605-615
Soundararajan, V., Zekovic, S., and Kovacevic, R. 2005. Thermo-mechanical model with adaptive boundary conditions for friction stir welding of Al 6061.
International Journal of Machine Tools & Manufacture,
45(14): p. 1577-1587.
Vilaca, P., Quintino, L., and dos Santos, J.F. 2005. iSTIR - Analytical thermal model for friction stir welding. Journal
of Materials Processing Technology, 169(3): p. 452-465.
Yuh, J. Chao, X. Qi, W. Tang, 2003. Heat transfer in friction stir welding experimental and numerical studies. Journal of
manufacturing science and engineering Vol. 125,
Zhu, X.K., Y.J. Chao, 2002. Effects of temperature-dependent
material properties on welding simulation. Computers and
Structures 80 967–976.
Zhu, X.K., Y.J. Chao, 2004. Numerical simulation of transient temperature and residual stresses in friction stir welding of
304L stainless steel. Journal of Materials Processing
Technology 146, 263–272.